Manual for Flash Butt Welding of Rails
Post on 16-Oct-2014
GOVERNMENT OF INDIA MINISTRY OF RAILWAYS MANUAL FOR FLASH BUTT WELDING OF RAILS 1996 RESEARCH DESIGNS AND STANDARDS ORGANISATION LUCKNOW-226011
MANUAL FOE FLASH BUTT WELDING OF RAILS
FOREWORD dian Railways, Alumino Thermic (A. T.) Welding, Flash Butt (Electric Resistance) Welding and Gas Pressure Welding processes are presently in use for welding of rail joints. Flash Butt Welding is being done on Zonal Railways departmentally, using Stationary Flash Butt Welding Plants of different makes. Mobile Flash Butt Welding Plants, capable of in situ Flash Butt Welding of rail joints, are also in operation on some of the Zonal Railways. The Code of Practice for Flash Butt Welding of Rails (tentative) was issued in January, 1972. Revision of this Code is being made to cover procedures for Flash Butt Welding of heavier and higher strength rails now used on Indian Railways and to incorporate the latest practices. This Code of Practice is being renamed as "Manual for Flash Butt Welding of Rails". MANUAL FOR FLASH BUTT WELDING OF RAILS 1. SCOPE 1.1 The manual gives details of the types and suitability of rails to be welded by stationary Flash Butt Welding Plant prewelding inspection, preparation of rail ends before welding, the general procedure of execution of welding and finishing of welded joints. It also defines geometrical tolerances for the finished joints and acceptance tests to ensure quality control. 1.2 Weld parameters for different rail sections/ chemistry have been prescribed by manufacturers and are unique to the particular welding plants. Should any change in these parameters be considered necessary, the same may be carried out in consultation with RDSO. 2. SELECTION OF RAILS TO BE WELDED 2.1 SECTION OF RAILS : Capacity of the individual plant will determine the heaviest section and type of rail that can be welded. New as well as released but serviceable rails of same type (section and metallurgy) shall only be welded together. Welding of rails of different sections metallurgy shall not be attempted. It is preferable that rails, rolled by the same manufacturer are welded together. Minimum length of old but serviceable rails for welding shall be 6 metres. 2.2 WELDING OF OLD RAILS : While welding old rails, it shall be ensured that only serviceable rails are welded. Old rails to be welded shall preferably be match marked before releasing from track to achieve maximum uniformity of profiles in weld zone.